Thermal conductivity reduction of crystalline silicon by high-pressure torsion
© Harish et al.; licensee Springer. 2014
Received: 24 April 2014
Accepted: 21 June 2014
Published: 28 June 2014
We report a dramatic and irreversible reduction in the lattice thermal conductivity of bulk crystalline silicon when subjected to intense plastic strain under a pressure of 24 GPa using high-pressure torsion (HPT). Thermal conductivity of the HPT-processed samples were measured using picosecond time domain thermoreflectance. Thermal conductivity measurements show that the HPT-processed samples have a lattice thermal conductivity reduction by a factor of approximately 20 (from intrinsic single crystalline value of 142 Wm−1 K−1 to approximately 7.6 Wm−1 K−1). Thermal conductivity reduction in HPT-processed silicon is attributed to the formation of nanograin boundaries and metastable Si-III/XII phases which act as phonon scattering sites, and because of a large density of lattice defects introduced by HPT processing. Annealing the samples at 873 K increases the thermal conductivity due to the reduction in the density of secondary phases and lattice defects.
Nanomaterials possess unique abilities to control thermal transport . Engineering the thermal properties of nanostructured materials have a promising application in the field of thermoelectrics. The thermoelectric system performance is evaluated by the dimensionless figure of merit, ZT = S 2 σT/k, where S is the Seeback coefficient, σ is the electrical conductivity, T is the temperature, and k is the thermal conductivity . To achieve higher ZT, lattice thermal conductivity of the thermoelectric material needs to be reduced without compromising the charge carrier mobility. Significant work has been done in recent years by using chemically distinct secondary phases either in the bulk form, or in the form of thin films, to reduce lattice thermal conductivity . The introduction of nanostructured interfaces to scatter phonons efficiently and thereby reducing the thermal conductivity of the material has yielded high ZT in thermoelectric devices [4–6].
From an engineering perspective, practical thermoelectric device requires a significant volume of material. To realize this objective, nanostructuring using ball milling followed by hot pressing was shown to have a significant reduction in the thermal conductivity of thermoelectric materials especially silicon [7–10]. Similarly, mechanical deformation using high pressure was adopted to improve the Seeback coefficient of Bi2Te3 and PbTe [11, 12].
Valiev et al.  demonstrated a novel technique using high-pressure torsion (HPT) to create a high density of lattice defects such as grain boundaries and dislocations on nanometer length scales . Ikoma et al. [14, 15], using HPT processing, reported detailed structural characterization of bulk crystalline silicon by X-ray diffraction spectroscopy, Raman spectroscopy, photoluminescence spectroscopy, and transmission electron microscopy and discussed the mechanism behind the nanograin formation in detail [14, 15].
Intrinsic high thermal conductivity of single crystalline silicon limits its application in thermoelectric systems. In this work, we show that bulk single crystalline silicon, when subjected to intense plastic strain through HPT processing, shows a dramatic reduction in room temperature thermal conductivity from its intrinsic single crystal value of 142 W m−1 K−1 to a low thermal conductivity of approximately 7.6 W m−1 K−1. The experimental thermal conductivity results are comparable to nanostructured silicon prepared by ball milling and spark plasma sintering approach reported in the literature [7–10]. Considering the widely adopted method of ball milling followed by plasma sintering in thermoelectric literature to form bulk samples, the current approach could be a promising alternative for such applications.
Single crystalline Si (100) wafers of size 5 × 5 mm2 and thickness 640 μm were subjected to HPT processing. Details of the HPT processing in Si was described elsewhere14. Briefly, the HPT facility comprises of upper and lower anvils made of tungsten carbide with flat bottomed spherical depressions to mount the test sample. During experiments, the test samples were placed in the lower anvil and the pressure was applied on the upper anvil. The HPT facility was operated at a pressure of 24 GPa (loading time approximately 7 s and unloading time approximately 2 s) and at room temperature. Torsional straining is achieved by rotating the lower anvil with respect to the upper anvil at a rotation speed of 1 rpm. HPT-processed samples with 0, 10, and 20 torsion cycles were prepared using this process. The samples were further annealed at 873 K for 2 h (0 and 10 torsion cycles) and 3 h (20 torsion cycles) in nitrogen atmosphere. We performed Raman and X-ray diffraction characterization independently and found that the experimental results were similar to previous literature results [14, 15].
Thermal conductivity measurements
The signals were analyzed assuming a unidirectional heat flow thermal model between the Al transducer film and the material . In brief, the analysis model accounts for thermal transport in layered structures from time periodic power source with a Gaussian intensity distribution . In our experiments, the modulation frequency of the pump beam is 150 kHz. The pump and probe beam spot sizes (1/e2 radius) are 37 μm and 14 μm, respectively. The Al transducer film thickness was measured as 135 nm using a profilometer.
Results and discussion
A possible reason for the dramatic reduction in lattice thermal conductivity is due to the decrease in grain size upon increasing plastic deformation. Our previous TEM investigations reported that the grain size of HPT samples reduces to as low as 10 nm during the HPT processing [14, 15]. Hao et al. theoretically calculated the thermal conductivity of nanograined silicon and showed that the thermal conductivity can be reduced to as low as 3 Wm−1 K−1 for a grain size of 10 nm which is comparable to the present experimental results. Phonon scattering at the nanograin boundaries increases as the grain size decreases which leads to the large reduction in the thermal conductivity. In addition, the presence of metastable Si-III/XII phases [14, 15] creates lattice mismatch which further scatters the acoustic phonons. Based on the literature, it is anticipated that the thermal conductivity decreases with decreasing grain size. The present experimental results show that the mean thermal conductivity of 10 torsion cycle case (lower grain size) is marginally higher than the 0 torsion cycle case (higher grain size). The reason behind this deviation is still unclear. Nevertheless, the experimental results clearly show an order of magnitude reduction in thermal conductivity upon HPT processing.
Annealing of the HPT-processed samples results in an increase of thermal conductivity especially for the 0 torsion cycle case. The effect of annealing becomes less pronounced for the 10 torsion cycles (33 Wm−1 K−1 after annealing) and 20 torsion cycles sample (16 Wm−1 K−1 after annealing) resulting in a smaller increase in thermal conductivity. The increase in thermal conductivity is due to the reverse transformation of the metastable phases to Si-I diamond phase and also due to reduction in the density of lattice defects such as vacancies, dislocations, and grain boundaries. Since our previous study reveals that no appreciable grain coarsening occurs during the annealing process [14, 15], the increase in thermal conductivity can be largely attributed to the reduction of the number of lattice defects; a contribution may also be present from the reverse transformation of metastable phases during annealing.
The present experimental results are comparable with the previous investigations in heavily doped p-type and n-type silicon. Existing literature results report a thermal conductivity reduction from approximately 100 W m−1 K−1 to 5 to 10 W m−1 K−1 at room temperature by varying the nature of alloy and the alloy concentration [7–10, 20]. The alloy typically used is germanium and the samples are prepared by ball milling for several hours to achieve small nanograin structures followed by hot pressing at a temperature of 1,473 K to form a bulk sample [7–10]. The advantage of present technique over ball milling lies in the fact that bulk samples are directly prepared in a short duration by HPT processing to obtain a dramatic reduction in thermal conductivity by a factor of approximately 20. Although, the present thermal conductivity of approximately 7.6 Wm−1 K−1 is still high for thermoelectric application, we anticipate that by using HPT processing combined with appropriate doping will result in further reduction of thermal conductivity of silicon and possibly other thermoelectric materials such as SiGe, Bi2Te3, and PbTe.
In summary, we demonstrated a novel way to reduce the lattice thermal conductivity of crystalline silicon by intense plastic strain through high-pressure torsion (HPT) at a pressure of 24 GPa. The grain boundary size decreases to nanoscale levels upon increasing the strain by HPT processing. The thermal conductivity of the HPT samples decreases to as low as approximately 7.6 Wm−1 K−1 due to the increase in phonon scattering at the nanograin boundaries. The present results introduce an efficient and irreversible way to make nanograin boundaries and provide a potential tool for the fabrication of thermoelectric materials with improved performance.
This work was supported in part by a Grant-in-Aid for scientific research from the MEXT Japan, in Innovative areas ‘Bulk Nanostructured Metals’ (Nos. 22102004, 2510278). SH was financially supported by postdoctoral fellowship from Japan Society of Promotion of Science (JSPS) for foreign researchers. MK acknowledges the support of JSPS KAKENHI 26289048. SH, MT, and MK acknowledge Takashi Yagi at AIST, Tsukuba for his helpful discussions on TDTR measurements.
- Cahill DG, Goodson KE, Majumdar A: Thermometry and thermal transport in micro/nanoscale solid-state devices and structures. J Heat Trans-T ASME 2002, 124: 223–241.View ArticleGoogle Scholar
- Goldsmid HJ: Thermoelectric refrigeration. New York: Plenum Press; 1964.View ArticleGoogle Scholar
- Nielsch K, Bachmann J, Kimling J, Bottner H: Thermoelectric nanostructures: from physical model systems towards nanograined composites. Adv Energy Mater 2011, 1: 713–731. 10.1002/aenm.201100207View ArticleGoogle Scholar
- Heremans JP, Jovovic V, Toberer ES, Saramat A, Kurosaki K, Charoenphakdee A, Yamanaka S, Snyder GJ: Enhancement of thermoelectric efficiency in PbTe by distortion of the electronic density of states. Science 2008, 321: 554–557. 10.1126/science.1159725View ArticleGoogle Scholar
- Kanatzidis MG: Nanostructured thermoelectrics: the new paradigm? Chem Mater 2010, 22: 648–659. 10.1021/cm902195jView ArticleGoogle Scholar
- Guin SN, Negi DS, Datta R, Biswas K: Nanostructuring, carrier engineering and bond anharmonicity synergistically boost the thermoelectric performance of p-type AgSbSe2-ZnSe. J Mater Chem A 2014, 2: 4324–4331.View ArticleGoogle Scholar
- Wang XW, Lee H, Lan YC, Zhu GH, Joshi G, Wang DZ, Yang J, Muto AJ, Tang MY, Klatsky J, Song S, Dresselhaus MS, Chen G, Ren ZF: Enhanced thermoelectric figure of merit in nanostructured n-type silicon germanium bulk alloy. Appl Phys Lett 2008, 93: 193121–1-3.Google Scholar
- Joshi G, Lee H, Lan YC, Wang XW, Zhu GH, Wang DZ, Gould RW, Cuff DC, Tang MY, Dresselhaus MS, Chen G, Ren ZF: Enhanced thermoelectric figure-of-merit in nanostructured p-type silicon germanium bulk alloys. Nano Lett 2008, 8: 4670–4674. 10.1021/nl8026795View ArticleGoogle Scholar
- Zhu GH, Lee H, Lan YC, Wang XW, Joshi G, Wang DZ, Yang J, Vashaee D, Guilbert H, Pillitteri A, Dresselhaus MS, Chen G, Ren ZF: Increased phonon scattering by nanograins and point defects in nanostructured silicon with a low concentration of germanium. Phys Rev Lett 2009, 102: 196803–1-4.Google Scholar
- Bux SK, Blair RG, Gogna PK, Lee H, Chen G, Dresselhaus MS, Kaner RB, Fleurial JP: Nanostructured bulk silicon as an effective thermoelectric material. Adv Funct Mater 2009, 19: 2445–2452. 10.1002/adfm.200900250View ArticleGoogle Scholar
- Ovsyannikov SV, Shchennikov VV: Pressure-tuned colossal improvement of thermoelectric efficiency of PbTe. Appl Phys Lett 2007, 90: 122103–1-3.View ArticleGoogle Scholar
- Ovsyannikov SV, Shchennikov VV, Vorontsov GV, Manakov AY, Likhacheva AY, Kulbachinski VA: Giant improvement of thermoelectric power factor of Bi(2)Te(3) under pressure. J Appl Phys 2008, 104: 053713–1-5.View ArticleGoogle Scholar
- Valiev RZ, Estrin Y, Horita Z, Langdon TG, Zehetbauer MJ, Zhu YT: Producing bulk ultrafine-grained materials by severe plastic deformation. JOM 2006, 58: 33–39.View ArticleGoogle Scholar
- Ikoma Y, Hayano K, Edalati K, Saito K, Guo QX, Horita Z: Phase transformation and nanograin refinement of silicon by processing through high-pressure torsion. Appl Phys Lett 2012, 101: 121908–1-4.View ArticleGoogle Scholar
- Ikoma Y, Hayano K, Edalati K, Saito K, Guo QX, Horita Z, Aoki T, Smith DJ: Fabrication of nanograined silicon by high-pressure torsion. J Mater Sci 2014. doi:10.1007/s10853–014–8520-z doi:10.1007/s10853-014-8520-zGoogle Scholar
- Cahill DG: Analysis of heat flow in layered structures for time-domain thermoreflectance. Rev Sci Instrum 2004, 75: 5119–5122. 10.1063/1.1819431View ArticleGoogle Scholar
- Carslaw HS, Jaeger JC: Conduction of Heat in Solids. 2nd edition. Oxford Oxfordshire New York: Clarendon Press; Oxford University Press; 1986.Google Scholar
- Fulkerso W, Moore JP, Williams RK, Graves RS, Mcelroy DL: Thermal conductivity electrical resistivity and seebeck coefficient of silicon from 100 to 1300°K. Phys Rev 1968, 167: 765–782. 10.1103/PhysRev.167.765View ArticleGoogle Scholar
- Hao Q, Zhu GH, Joshi G, Wang XW, Minnich A, Ren ZF, Chen G: Theoretical studies on the thermoelectric figure of merit of nanograined bulk silicon. Appl Phys Lett 2010, 97: 063109–1-3.Google Scholar
- Stein N, Petermann N, Theissmann R, Schierning G, Schmechel R, Wiggers H: Artificially nanostructured n-type SiGe bulk thermoelectrics through plasma enhanced growth of alloy nanoparticles from the gas phase. J Mater Res 2011, 26: 2459–2459. 10.1557/jmr.2011.311View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.